Accepted Manuscript Title: Nanoporous membranes with cellulose nanocrystals as functional entity in chitosan: Removal of dyes from water Author: Zoheb Karim Aji P. Mathew Mattias Grahn Johanne Mouzon Kristiina Oksman PII: DOI: Reference:
S0144-8617(14)00624-9 http://dx.doi.org/doi:10.1016/j.carbpol.2014.06.048 CARP 9013
To appear in: Received date: Revised date: Accepted date:
19-4-2014 7-6-2014 11-6-2014
Please cite this article as: Karim, Z., Mathew, A. P., Grahn, M., Mouzon, J., and Oksman, K.,Nanoporous membranes with cellulose nanocrystals as functional entity in chitosan: Removal of dyes from water, Carbohydrate Polymers (2014), http://dx.doi.org/10.1016/j.carbpol.2014.06.048 This is a PDF file of an unedited manuscript that has been accepted for publication. As a service to our customers we are providing this early version of the manuscript. The manuscript will undergo copyediting, typesetting, and review of the resulting proof before it is published in its final form. Please note that during the production process errors may be discovered which could affect the content, and all legal disclaimers that apply to the journal pertain.
Nanoporous membranes with cellulose nanocrystals as
functional entity in chitosan: Removal of dyes from water
Zoheb Karim1, 2, Aji P. Mathew1*, Mattias Grahn2, Johanne Mouzon2,
Kristiina Oksman1, 1
Division of Materials Science, Luleå University of Technology
97187, Luleå, Sweden 2
Department of Civil, Environmental and Natural Resources Engineering,
Division of Sustainable Process Engineering
97187, Luleå, Sweden
Fully biobased composite membranes for water purification were
fabricated with cellulose nanocrystals (CNCs) as functional entities in chitosan
matrix via freeze drying process followed by compacting. The chitosan (10 wt
%) bound the CNCs in a stable and nanoporous membrane structure with
thickness of 250 -270 m, which was further stabilized by crosslinking with
gluteraldehyde vapors. Scanning electron microscopy (SEM) studies revealed
well-individualized CNCs embedded in a matrix of chitosan. Brunauer,
Emmett and Teller (BET) measurements showed that the membranes were
nanoporous with pores in range of 13-10 nm. In spite of the low water flux
(64Lm-2h-1), the membranes successfully removed 98%, 84% and 70%
23 24 25 26 27
Ac ce p
respectively of positively charged dyes like Victoria Blue 2B, Methyl Violet 2B and Rhodamine 6G, after a contact time of 24 hrs. The removal of dyes was expected to be driven by the electrostatic attraction between negatively charged CNCs and the positively charged dyes. Key words: cellulose nanocrystals, chitosan, nanoenabled membranes, dye removal, water purification, adsorption
*Corresponding author: Aji P Mathew
Division of Materials Science, Luleå University of Technology
97187, Luleå, Sweden
Ph +46-92493336, email: [email protected]
33 1 Page 1 of 25
1. Introduction Shortage and contamination of global drinking water calls for the
development of highly effective water purification techniques. The removal of
various pollutants such as heavy metals, dyes, pesticides, herbicides and
other industrial as well as agricultural wastes from wastewater has become a
critical issue due to their adverse effects on human health and environment.
(Lin et al., 2011, Huang et al., 2011)
Recently, advances in nano scale science and engineering suggest
that many of the current problems involving water quality could be greatly
diminished by using nano-materials due to their good adsorption efficiency,
higher surface area and greater active sites for interaction with pollutants
(Diallo et al., 2005, Dhermendra et al., 2008). Several studies have shown the
effectiveness of nano-enabled membranes for cleaning industrial wastewater
such as fish-meal wastewater, solutes from etching processes, wastewater
from textile industry etc (Dhermendra et al, 2008, Ma et al., 2011a). However
these technologies poses significant challenges in term of limited availability
of nano materials, cost effectiveness and environmental concerns.
Polysaccharides, such as cellulose and chitin, are among the most
abundant biomaterials on earth, having low cost, environmental friendly,
renewable and biodegradable properties (Samir et al., 2005; Muzzarelli et al.,
2007; 2012). By intelligent processing techniques and properties they could
56 57 58 59 60 61
Ac ce p
be used as classical nano-reinforcements/functional elements in polymers for the preparation of membranes (Ma et al., 2011a; Ma et al., 2012). Cellulose nanocrystals (CNCs) and nanofibers isolated from bioresources have been studied as reinforcements and/or functional entity in various synthetic and natural polymer matrices and for different applications. (Samir et al., 2005; Petersson et al., 2007; Kvein et al., 2007: Saxena et al., 2009; Mikkonen et al., 2010; Mathew et al., 2012; Narges et al., 2014). Recently, Ma et al. (2012)
developed a membrane, where ultrafine CNCs were infused into an
electrospun polyacrylonitrile nano-fibrous scaffold supported by mechanically
strong polyethylene terephthalate nonwoven substrate. The impregnated
CNCs possessed very high negative surface charge density and thus
provided high adsorption capacity to remove positively charged species, viz.
crystal violet dye. Thus, adsorption has been proved to be an economical 2 Page 2 of 25
method for the treatment of wastewater contaminants. Now-a-days, almost all
the adsorbents developed for removal of contaminants rely on the surface
interactions and therefore the functional groups available on the surface of the
adsorbents played an important role in determining the effectiveness,
capacity, selectivity and reusability of the adsorbent material (Wesenberg et
al., 2003; Liu et al., 2005; Xiao et al., 2010 Dural et al., 2011). Furthermore
large surface area and abundance of adsorption sites are essential for
adsorption and removal of the contaminants from wastewater (Li et al., 2005a;
Li et al., 2005b; Liu et al., 2014)
In the current study CNCs having required functional groups (SO3-
and/or COO-) (Liu et al., 2014) for the removal of targeted dyes by
electrostatic interaction, are used as functional entity for the fabrication of
composite membranes. Chitosan is used as the matrix phase. Though
chitosan is traditionally used in water purification, it is mostly effective towards
negatively charged acidic dyes due to functional group present on chitosan (-
NH2+) (Crini, 2006; Bingei et al., 2013). However, the water permeability and
water stability of chitosan in different pH conditions, especially after
crosslinking will be of advantage in fabricating water-cleaning membranes
(Mathew et al., 2009). A very simple technique, freeze-drying was applied for
the fabrication of composite membranes. The biggest advantage with process
was fabrication of a loose and non-aggregated network, which is expected to
90 91 92 93 94 95
Ac ce p
provide easy availability of surface groups on CNCs as adsorption sites for contaminants. High concentration of functional entity (CNCs) was used with an aim to have high process efficiency. The process method as well the matrix used is expected to make the surfaces of functional entity readily available for interaction with contaminants in water. ATR-FTIR analysis was performed to understand the basic binding
parameters with CNCs and matrix, chitosan. SEM and BET techniques were
used to characterize the membrane morphology and pore structure. Flux and
mechanical performance of the composite membranes was also determined.
Three positively charge dyes (Victoria Blue 2B, Methyl Violet 2B and
Rhodamine 6G) that are real concern in industrial wastewater were chosen for
the study. It may be noted that these dyes are of industrial and environmental
relevance as (i) according to the Swedish Environmental Protection Agency, 3 Page 3 of 25
the selected dyes came under section “very hazardous” contaminants, (ii) the
three selected dyes having negative impact in southern Europe, especially in
Spain and (iii) these dyes had very harmful effects not only on human but on
aquatic life also.
Non-dried cellulose residue (sludge) from dissolving cellulose
production was obtained from Domsoj Fabriker AB, Ornskoldsrik mill,
Sweden, with a water content of 50 wt%. Based on the data from the material
supplier, the chemical composition of the used sludge was, cellulose content
(95%), hemicellulose (4.75%) and very low content of lignin.
Chitosan from shrimp shells (medium molecular weight having deacetylation
value ≥ 75.5% and viscosity, 20-300 cps); Polyethylene glycol (PEG 2000)
and gluteraldehyde (50%) were purchased from Sigma-Aldrich (USA). Acetic
acid (96 %) and sulfuric acid (98 %) were supplied by VWR (BDH, France).
chemicals were used without any purification.
Sludge was used as received without any pretreatments and all
2.2. Processing Methods
2.2.1. Isolation and characterization of CNCs
CNCs were prepared by acid hydrolysis of non-dried cellulose residue
123 124 125 126 127 128 129
Ac ce p
(sludge) following the sulfuric acid hydrolysis as procedure by Bondeson et al. (2006), with minor modifications. The sludge was hydrolyzed with 63.5% sulfuric acid for 105 min at 45 oC. The resulting suspension underwent a series of centrifugation, washing with deionized water, and sonication steps to collect the CNCs in the supernatant. This was neutralized by dialysis and stored until further use in the form of aqueous suspensions. Isolated CNCs were concentrated by dialysis against PEG to a concentration of 4.2 wt% prior
to use for membrane fabrication. The yield of CNCs from the process was
17% with respect to the used cellulose residue weight.
2.2.2.Preparation and crosslinking of nanocomposite membrane
Chitosan was first dissolved in 2 wt% acetic acid followed by addition of
deionized water to form a solution of 1 wt%. The concentrated CNCs were 4 Page 4 of 25
mixed with chitosan solution in 9:1 ratios and the total concentration of mix
was 2 wt%. The mixture of chitosan and CNCs were casted into petri plates
and put into freezer to solidify. The solidified mixture was freeze-dried in a
ALPHA 2-4 LD Plus freeze dryer at -75 oC for 24 h. After freeze-drying, the
prepared porous composites were pressed between aluminum plates in a
compression molding machine (Fontune Presses, Elastocon, Sweden) without
heating to obtain compacted membranes. Same procedure was followed for
the preparation of native chitosan (0.2 wt%), used as control. Crosslinking
was performed by placing the compacted membranes in a desiccator with
gluteraldehyde vapours; 25% of gluteraldehyde at room temperature for 48 h
was used. In uncross-linked as well as cross-linked membranes the final CNC
concentration was 90 wt %.
2.3.1. Morphology and pore structure
Atomic Force microscopy (AFM) was analysed using a Veeco Multi
Mode instrument equipped with Nanoscope V controller. A droplet of the
aqueous CNCs suspension (0.2 %) was dried on a freshly cleaved mica
surface prior to AFM examination. AFM images were captured in tapping
mode using coated Si probes at a resonance frequency of 70 kHz and having
a spring constant of 1-5 N/m.
157 158 159 160 161 162 163
The morphology of uncross-linked and cross-lined membrane was
Ac ce p
examined at high magnification using MAGELLAN 400, SEM (FEI Company). The membranes were fractured and sputter coated with tungsten. The films were observed in the SEM at an acceleration voltage of 20 kV. 2.3.2. Chemical characteristics A Bruker IFS 66v/S spectrometer equipped with liquid nitrogen cooled
mercury–cadmium–telluride (MCT) detector and a vertical ATR-FTIR accessory was used for collecting infrared data. Both single beam background
and sample spectra were acquired by averaging 500 scans at a resolution of
4 cm−1. Spectra evaluation was performed using the Bruker Opus 4.2
5 Page 5 of 25
Specific surface area and pore size of fabricated composites were determined
by N2 adsorption using BET method with sample-degassed instrument
(Micromeritics ASAP 2000, Sweden) at 100 oC for 24 h in dry N2 flow.
2.3.4. Mechanical properties The tensile tests of the uncross-linked and cross-linked membranes were
performed using a universal testing machine, Shimadzu Autograph AG-X
(Japan), with a load cell 1kN and the gauge length was 20 mm. Test
specimens were 5 mm and 0.25 mm in nominal width and thickness as
measured by digital caliper for membrane. The samples were preloaded with
1 N before starting the tensile test. The samples were stretched with 2mm/min
crosshead speed until failure. The stress-strain curves were plotted from the
measured load and samples extension. The stress is defined as σ = F/(AoLo)
and the train as ε = In (L/Lo), where F is the instantaneous force, Ao is the
initial sample cross section, and Lo is the initial sample length. The elastic
modulus was calculated from the initial part of the slop from stress-strain
curve. At least five test samples were tested for each material and the
average values were presented.
2.3.5. Flux measurement
A dead-end stirred cell filtration system connected with a N2 gas cylinder was
used to evaluate the flux performance of the composite membranes. All
experiments were carried out using a filtration test cell, Dead End Cell
190 191 192 193 194 195 196
Ac ce p
(Sterlitech HP4750 Stirred cell, U.S.A) with a capacity of 300 ml. The effective area of the membrane was 17.3 cm2. The operation pressure (0.196 MPa) in the system was maintained by nitrogen gas. Composite membranes were conditioned in water for one day prior to measurement of water flux. The amount of solvent passing through the membranes under applied pressure within a fixed time interval was used to calculate water flux (Lm-2h-1MPa-1). The water flux (F) was calculated using formula equation 1. F = Vo (L)/To (h) x Ao ( m2 )x Po (MPa)…………………………..(1)
where Vo is volume of solvent that passed through the membrane, To is time
of measurement, Ao is effective membrane area and Po is applied pressure.
It was not possible to measure the water flux of pure chitosan as the freeze-
dried structure was completely destroyed because of dipping chitosan
membrane in water before measurement of water flux. 6 Page 6 of 25
2.3.6. Evaluation of dye removal efficiency The quantitative analysis of untreated and treated model wastewater was
determined by U.V-visible spectrophotometer (Perkin Elmer, Lambda 2S,
Sweden). The percentage removal was calculated by formula as given below
where Ao is absorbance of treated dye solution with chitosan membrane and
At is absorbance of treated dye solution with composite membrane. The
absorbance of each dye was recorded at their λmax, determined by U.V-visible
spectrophotometer. The optical absorbance of dyes, Methyl Violet 2B,
Rhodamine 6G and Victoria blue 2B at 581, 526 and 616 nm respectively
were monitored by U.V-visible spectroscopy to determine the percentage
removal of dyes. Table 1 summarizes the chemical structure and other
parameters of the used dyes.
Core structure of dyes
Ac ce p
Table 1: Information about targeted dyes
7 Page 7 of 25
Some screening experiments on the effect of pH, incubation time and
doses of dyes with uncross-linked hybrid membrane only, were performed to
determine the best conditions to study the maximum removal efficiency of the
prepared hybrid membranes.
Stock solution of model wastewater was prepared by adding dyes (10
mg/L) in deionized water. The 1mg/L of model wastewater was used with
uncross-linked and cross-linked membranes. Composite membranes cut into
30x20mm of pieces were incubated for 24 h in solution of pH 5.01 at room
temperature (23±2) with stirring. The model wastewater treated with 0.2%
chitosan was taken as control for determination of percentage removal by
composites membranes using formula mentioned above. All experiments
were performed in dark to prevent the photo-degradation.
3. Results and Discussion
Ac ce p
3.1. Characteristics of Cellulose nanocrystals
231 232 233
Fig. 1: a) AFM image of isolated CNCs and b) flow birefringence of CNCs suspension, observed between two crossed polarizers.
8 Page 8 of 25
The AFM images in Figure 1 show the presence of isolated cellulose
nanocrystals in the nanometer scale. CNC displays rod-like shape with
diameters in the range of 6 - 10 nm, as measured by Nanoscope V software.
The nanocrystal dimension agrees with our earlier reports of CNC prepared
with same isolation process, by Kvien et al. (2005) to be of 5±2 nm width and
length of 210±75 nm. The flow birefringence (Fig. 1b) of aqueous
nanocrystals when viewed under cross-polarized light also supported the
existence of CNCs (Araki et al., 2000; Bondeson et al., 2006).
Crystallinity of isolated CNCs was 70%, and had a surface charge density of
230 μmol/g as calculated from the conductometric titration curve. The Z-
potential of CNCs remained negative in the pH range of 3-12, as reported in
our previous published work (Liu et al., 2014).
3.2. Morphology of prepared composite membrane
Ac ce p
Fig. 2: SEM images of prepared membranes showing a) layered structure of
uncross-linked membranes and b) the detailed view of the membrane
showing the homogeneous dispersion of CNCs in the matrix c) the layered
structure of crosslinked membranes (d) the detailed view of the CNCs 9 Page 9 of 25
dispersed in the crosslinked matrix. In inset images shows one layer of the
uncross-linked membrane (inset b) cross-linked membrane (inset d),
comparing the compactness before and after crosslinking.
Figure 2a and 2c shows the overview images for uncross-linked and cross-linked nanocomposites membranes, respectively. The thickness of the
membrane was estimated to be in the range of 250 -270m. In both cases
layered structure was observed, which is expected to have formed during
compacting of freeze dried material. Another reason is the high concentration
of used CNCs. Recently, Han et al. (2013) reported the concentration
dependent mechanism for lamellar or fiber structure morphology of
nanocellulose through freeze-drying. According to their results, at low
concentration (0.05 wt%), nanocelluloses were self-assembled into oriented
ultrafine fibers but at high concentration (0.5 and 1 wt%), the lamellar
structured foam composed of aligned thin membrane layers. Similar layered
structures were reported for freeze-dried membranes from nanocellulose
fibers also (Gebald et al., 2011). The images also show that the cross-linked
system is slightly denser than the uncross-linked ones.
Figure 2b and 2d shows the detailed view of the uncross-linked and cross-
linked nanocomposite membranes. The detailed image shows the
nanoscaled morphology of the membranes while the inset image shows one
Ac ce p
chitosan matrix even at high concentration indicates positive interaction
between chitosan matrix and CNCs. It may be considered that the CNCs are
bound together in a three dimensional network by chitosan chains. In the
current study also we have the advantage of the common solvent and further
more the processing methods used, viz freeze-drying is considered as an
efficient route to limit aggregation of nanocellulose.
272 273 274 275 276
layer of the membranes. The SEM images of uncross-linked membranes showed that CNCs were regularly dispersed within the chitosan forming a network of CNCs with absence of visible agglomerates (Fig. 2b). Cross-linked nanocomposite membrane also shows uniform dispersion of CNCs within the chitosan network in random orientation but little tight network due to the crosslinking with glutaraldehyde (Fig. 2d). The good dispersion of CNCs in
10 Page 10 of 25
Gebald et al. (2011) recently reported cellulose nanofibers membrane for the adsorption of CO2 prepared by freeze-drying. In this study, SEM images of
prepared membrane revealed single irregularly distributed cellulose fibrils
attached to the cellulose sheet, after freeze-drying and aggregation of
cellulose nanofibrils to form sheet upon freezing was recorded. It is expected
that in the current study the combination of the choice of matrix, and the
processing method have positively impacted the homogeneous dispersion
and distribution of CNCs. The infused and well-dispersed CNCs within the
chitosan network offer several advantages in membrane technology as high
surface-to-volume ratio that makes them high adsorption efficiency towards
3.3. Evaluation of molecular level interactions
To understand the interaction between the chitosan polymer and CNCs in the composite membrane, FTIR spectroscopy of the samples was
performed using the ATR (Attenuated Total Reflection) technique (see
supplementary data for the spectrum). The spectra of chitosan and CNCs
were typical to spectra previously reported on these substances (Pavia et al.,
2002), The main bands in the spectrum of chitosan were located around 1643
and 1558 cm-1. The first band was for C=O stretching of acetyl group and the
second band was the N-H bending vibrations of amide and amine groups. The
306 307 308 309 310 311
Ac ce p
bands at 1070 cm-1 and 1030 cm-1 were due to the C-O stretching vibration, whereas the broad band at 3100-3400 cm-1 was on behalf of O-H and N-H stretching vibrations. The peaks 1375 cm-1 and 1350 cm-1 were indicating – CH3 group of N-acetyl glucosamine residue and –CH2 groups, respectively. All mentioned peaks were in the agreement of previous reported works. (Shigemasa et al.,1996; Brown et al., 2011), In pure CNCs, the broad band centered at ca 3400 cm-1 was related to
O-H stretching vibration. The bands at 2893 cm-1 and 1431 cm-1 were
characteristic of C-H stretching and bending of –CH2 groups, respectively,
where the peaks at 1160 cm-1 and 1070 cm-1 were typical to the saccharide
structure as mentioned and summarized by Strand et al. (2010).
The spectrum of nanocomposite membrane shows characteristic
bands of both raw materials (CNCs and chitosan). The saccharide and the C11 Page 11 of 25
H stretching bands at 1160 cm-1 and 1070 cm-1 in CNC could be observed in
the spectrum of the nanocomposite membrane as well as bands related
chitosan viz. the C=O stretching and N-H bending bands at 1643 cm-1and
1558 cm-1, respectively. Given the structure of chitosan and CNCs and the
processing method used, the formation of hydrogen bonds between theses
compounds is less expected. Both electrostatic and dispersion forces may
however also play a part in keeping the composite membranes together. In
the case of cross-linked nanocomposite membrane, a relatively weak
characteristic absorption band 1550-1600 cm-1 can be assigned to the Schiff
base (Brown, 2011).
It is expected that similarities between the chemical and molecular structures of CNCs and chitosan enable high affinity between both polymers.
Generally, CNCs-chitosan intermolecular interaction are based on H-bond,
Van der Waals forces, ionic and/or covalent bonds, depending on the
processing route (Al-Ghouti et al., 2010). In this study, the process of hybrid
membrane fabrication was freeze-drying which was directly responsible for
the absence of hydrogen bonding, resulting loose network between CNCs and
matrix, chitosan. Thus, the bonding between functional entity, CNCs and
matrix, chitosan was predominantly by electrostatic interaction, dispersive
forces and chemical bonds. The isolation of CNCs with acid hydrolysis
(H2SO4) introduced sulfate groups (replaced by aldehyde) onto the surface of
340 341 342 343 344 345
Ac ce p
CNCs. So there was a high chance for introduction of electrostatic interaction within the CNCs and chitosan. According to the Strand et al. (2010), the binding of cellulose on chitosan depends only on two factors; (i) a satisfactory amount of anchoring sites especially, introduction of functional groups in/on cellulose, onto which chitosan could bind and at the same time (ii) satisfactory free amino groups of chitosan, and both these binding mechanism are applicable in the current system.
346 347 348 349
12 Page 12 of 25
membrane Table 2: BET results of uncross-linked and cross-linked membranes Type BET surface Average pore area (m2/g)
3.4. Measurement of pore size and surface area of composite
The BET results were summarized in Table 2. The BET surface areas of uncross-linked and cross-linked composite membrane were 3.1 and 2.9
m2/g, respectively. This surface area is lower than some earlier reports on
freeze dried nanocellulose membrane structures The freeze-dried NFC
showed a BET surface area of 26.8 m2/gm where as the amine functionalized
NFC showed 7.1 m2/gm (Gebald et al., 2011). In the current freeze-dried
structures, the compacting process was considered to be responsible for the
relatively lower surface area, recorded in BET measurements. The pore sizes
of membranes were also determined by same technique and were found to be
17 and 13nm for uncross-linked and cross-linked composite film, respectively.
From these results it was confirmed that the crosslinking decreases surface
area as well as pore size of nano-enabled membrane and thereby can be
considered as more compacted than the uncrosslinked one. This data also
367 368 369 370 371
Ac ce p
supports the SEM observations. The decrease of pore size was also reported by Gebald et al. (Gebald et al., 2011) when amine was loaded in composite membrane. Recently, Ma et al. ( Ma et al., 2012, Ma et al., 2011b) showed that pore size of CNCs nano-enabled membrane decreased with increased concentration of functional materials. 3.5. Mechanical stability
The mechanical properties of uncross-linked and cross-linked nanocomposite
were summarized in Table 3.
Table 3: Mechanical testing results of uncross-linked and cross-linked
13 Page 13 of 25
Strain at break
377 The tensile strength of the uncross-linked membrane was 0.98 MPa where as
that of cross-linked ones was 1.1 MPa. The modulus values increased from
128 MPa to 318 MPa after crosslinking. The strain at break showed no
difference before and after crosslinking. The low mechanical performance in
is attributed to the fabrication method used viz. freeze drying, that restrict the
hydrogen bonding between CNCs as well as with the matrix phase and
thereby resulting in a loosely bound structure. This processing method used is
therefore not the best option in terms of mechanical performance but is good
for having well dispersed nanoparticles and a porous structure. Further more,
the positive impact of crosslinking on mechanical properties was significant
especially with respect to modulus of elasticity.
The permeability of pure water through the composite nanostructured
membrane was 64 Lm-2h-1MPa-1. The flux values of tested membrane first
decreased slowly during the filtration process because of the scaffold
Ac ce p
3.6. Flux measurement of composite membranes
394 395 396 397 398 399
compaction. It was found that the stable permeation flux of composite membrane was reached after 1 h of operation. Ma et al. (2011a) had reported that the flux through a microfiltration membrane using CNCs as infused entity within PAN nanofibrous scaffold was 59 Lm-2h-1 KPa-1 and much higher than commercial membrane, GS0.22 (25 Lm-2h-1KPa-1). The freeze-dried nanocomposite membranes presented in the current work showed lower water permeation flux as compared to both reported membranes; probably
due to the high membrane thickness (250-270 m). However, in the current
case low flux is not considered as a disadvantage as increased contact time
3.7. Dyes removal
14 Page 14 of 25
The pH conditions, time of incubation and the pollutant concentrations are considered as important parameters that affect the efficiency of dye
adsorption. The effect of pH on the percentage of dyes removal from aqueous
model wastewater by composite membranes is illustrated in Figure 3.
Fig. 3. Graph showing the effect of pH and incubation time on the adsorption
of Methyl Violet, Rhodamine 6G and Victoria Blue
Ac ce p
decreases with an increase in the solution pH, the electrostatic attraction
between positively charges dyes and the surface of adsorbent (composite
membrane) is lowered, which may results in an decrease in the rate of
adsorption. The table shows the maximum percentage removal of dyes from
model wastewater at pH 5.01 and the removal percentage decreases with the
increase in pH values. The negative zeta potential of CNC and its
411 412 413 414 415
Effect of pH was determined by incubation of hybrid composite
membranes for 24 h with dyes solutions (1mg/L) having pHs 5.01, 7.02 and 9.02 at room temperature. In these experiments, the initial solution pH was adjusted to the desired value (pH value: 5-9) using either 1M HCl or 1M NaOH solutions. Variation in pH can affect the surface charge potential of the adsorbent and degree of ionization. As the surface charge potential
15 Page 15 of 25
dependence on pH was reported in our earlier study (Liu et al 2014). The
functionality of the membranes showed a direct dependence on the zeta-
potential of CNC suggesting that surface characteristics of CNC determine the
efficiency of adsorption.
The optimum value of pH was chosen as 5.01 and used in the study of the
effect of incubation time. The incubation times were varied between (12-36 h)
in dyes solutions (1mg/L, pH 5.01) at room temperature. The results are
shown in Figure 3. Optimal removal efficiency of composite membranes was
observed for 24 h of incubation time for all dyes.
The optimal values of incubation time (24 h) for all dyes and pH were further
used for the determination of the dyes doses for the experiments. Table 6
shows the adsorption capacity of fabricated composite membrane at different
concentrations. The adsorption capacity of composite membrane decreased
with increase in the concentration of dyes. Approximately, complete removal
(98%) of Victoria Blue 2B was recorded at 1mg/L concentration. It was
inferred that 1mg/L was the upper limit of dye dosage to evaluate the
percentage removal of dyes.
Table 4: Effect of dose of dyes on the removal of dyes
Ac ce p
pH and incubation time were used
Composite membranes were of 30 x 20 mm in size, Standardized values of
3.7.1. Removal of dyes with standardized parameters
Targeted dyes having positively charges species were used to
determine the adsorption effectiveness of uncross-linked and cross-linked
membrane. It was noted that both the membranes were stable in water during 16 Page 16 of 25
the experiments and the cross-linked system showed enhanced dimensional
stability which may be attributed to the binding of CNCs in a three dimensional
network of chitosan polymer chains. The uncrosslinked composites showed
slight swelling after contact with dye solutions but was not significant enough
to affect the performance.
453 Table 5: Effect of composite membrane on removal of dyes
Percentage removal of dyes Uncross-linked
Methyl Violet 2B
Victoria Blue 2B
Types of dyes
The percentage removal was calculated as mentioned in equation 1. The
solution treated with 0.2% chitosan membrane was used to measure the
value of control
d te Ac ce p
17 Page 17 of 25
ip t cr us an M
Fig. 4: A schematic representation of experiment shows the naked eyes
detection of removal efficiency of cross-linked composite membrane. a)
Photograph of the membrane, water before and after adsorption test for b)
methyl violet c) Rhodamine 6G and d) Victoria Blue and the membranes with
respective adsorbed dyes
Ac ce p
Rhodamine 6G irrespective of the crosslinking. It is also noted the crosslinking
did not have significant impact on the adsorption capability of the membranes.
This suggests that the matrix do not influence the adsorption efficiency as it is
a minor component (10 wt %) and also due to presence of same charge
(positive charge) on surface. This also indicates that the CNCs, which are
465 466 467 468
Table 5 summarizes the dyes removal reached at 24 h by uncross-
linked and cross-linked membranes for all dyes solutions. Fig. 4 gives the visual illustration for the removal of dyes by crosslinked composite membranes. It was found that all the dyes showed good adsorption on the membranes being the highest for Victoria blue followed by Methyl violet and
18 Page 18 of 25
loosely bound by the matrix are well individualized due to freeze drying
method used and act as the functional entity for capturing the dyes. The adsorption of dyes may be driven by (i) specific characteristics of dyes (charge, charge potential, functional groups responsible for binding with
adsorbent etc.) and (ii) specific affinity of the dyes for the adsorbent. These
kinds of attractions may be predominantly of electrical, van del Waals or
chemical nature leading to adsorptions driven by dispersion forces,
complexation, hydrogen bond or electrostatic interaction (Al-Ghouti et al.,
2010) CNCs with high negative charges on the surface (as confirmed by zeta-
potential values) and targeted dyes having positively charges as shown in
Table 1., which leads to electrostatic interaction between the pollutants (dyes)
and fabricated composite membranes. Fig. 5 further illustrates the
electrostatic attraction between dyes molecules and the cellulose-O- on the
membrane surface. Other researchers also in dye removal reported similar
mechanisms from water.
Fig. 5: A schematic representation of the mechanisms of binding of the dyes
with CNCs via a) hydrogen bond formation and b) electrostatic
Ac ce p
Kaewprasit et al. (Kaewprasit et al 1998) showed the adsorption of methylene blue dye on cotton fiber (cellulose structure) due to the formation of 19 Page 19 of 25
stable ionic bonds between membrane surface and dyes molecules, which
prevent dyes molecules from being eluted from the membrane surface. In
another study a micro-nano structured poly(ethersulfones)/
poly(ethyleneimine) nanofibrous membrane was fabricated and utilized as an
adsorbant for three anionic dyes viz, Sunset Yellow, Fast Green and
Amaranth (Min et al 2012). These researchers had further demonstrated that
the species of charge present on the surface of composite determined the
maximum adsorption of positively charged dye due to the interaction of
positive and negative charges.
Isolated CNCs isolated from low cost sludge from industrial cellulose
production was used as functional entity for the preparation of fully biobased
nanocomposite membranes with chitosan as a matrix. Crosslinking of
nanocomposite showed positive impact on mechanical stability and
dimensional stability in moist environment and also resulted in slight
decrease in surface area and pore size. The pore diameter was found to be
in 13-17 nm range and classifies these membranes as ultrafiltration
membranes. The higher efficiency for the removal of dyes was observed,
being the highest for Victoria blue (98%), followed by Methyl violet (90%)
and Rhodamine 6G (78%). Two mechanisms were proposed for dyes
noted that freeze-drying adversely affected the mechanical performance of
the membranes and will be addressed in the future studies.
The authors gratefully acknowledge the financial support by European
Commission, under NanoSelect project, EU FP7-NMP4-SL-2012-280519.
517 518 519 520 521
Ac ce p
adsorption onto the membrane, hydrogen bonding and electrostatic interaction. Further more, the membranes showed low flux (64Lm-2h-1MPa); which support the usefulness of composite membranes as adsorbents. The high efficiency of the membranes, in terms of adsorption was attributed the freeze drying process used, which resulted in well individualized CNCs which act as functional entities which were loosely bound together by chitosan polymer chains locked in a 3D network via crosslinking. It may however be
20 Page 20 of 25
Iftekhar Uddin Bhuiyan, Luleå University of Technology, is acknowledged for
support with BET.
530 6. References
532 533 534 535 536 537 538 539 540 541 542 543 544 545 546 547 548 549 550 551 552 553 554 555 556 557 558 559 560 561
Al-Ghouti M.A., Li J., Salamh Y., Al-Laqtah N., Walker G., Ahmad M.N.M. (2010) Adsorption mechanism of removing heavy metals and dyes from aqueous solution using date pits solid adsorbent. J. Hazardous Mater. 176, 510-520.
565 566 567
Araki J., Wada M., Kuga S., Okani T. (2000) Birefringent glassy phase of a cellulose microcrystal suspension, Langmuir, 16, 2413-2415.
Bingjie L., Dongfeng W., Guangli Y., Xianghong M. (2013) Adsorption of heavy metal ions, dyes and proteins by chitosan composite and derivatives-A review. J. Ocean Uni. China,12, 500-508.
Bondeson D., Mathew A., Oksman K., (2006) Optimization of isolation of nanocrystals from microcrystalline cellulose by acid hydrolysis. Cellulose, 13 171-180.
Brown E.E., Laborie M.P., Zhang J. (2011), Gluteraldehyde treatment of bacterial cellulose/fibrin composite: impact on morphology, tensile and viscoelastic properties. Cellulose, 4, 1-11.
Crini G. (2006) Non-conventional low-cost adsorbents for dye-removal: a review, Bioresources Technology, 97, 1061-1085. Dhermendra K.T., Behari J., Prasenjit S.(2008) Application of nanoparticles in wastewater treatment. WASJ, 3, 417-433.
Ac ce p
562 563 564
Diallo M.S., Christie S., Swaminathan P., Johnson J.H., Goddard W.A (2005) Dendrimer enhanced ultra-filtration recovery of Cu (II) from aqueous solutions using Gx-NH2-PAMAM dendrimers with ethylene diamine core, Environ. Sci. Technol. 39, 1366-1377. Dural M.U., Cavas L., Papageorgiou S.K., Katsaros F.K. (2011) Methylene blue adsorption on activated carbon prepared from Posidoniaoceanica (L.) dead leaves: kinetics and equilibrium studies, Chem. Eng. J. 168, 77–85. Gebald C., Wurzbacher J.A., Tingaut P., Zimmermann T., Steinfeld A. (2011), Amines-based nanofibrillated cellulose as adsorbent for CO2 capture, Environ. Sci. Technol. 45, 9101-9108.
568 569 570
Huang C.H., Chang K.P., Ou H.D., Chiang Y.C., Wang C.F. (2011) Adsorption of cationic dyes onto mesoporous silica, Micro. Meso. Matt., 141,102–109. 21 Page 21 of 25
Jingquan Han., Chengjun Zhou., Yiqiang Wu., Fangyang Liu., Qinglin Wu., (2013). Self assembling behavior of cellulose nanoparticles during freezedrying: Effect of suspension concentration, particle size, crystal structure and surface charge, Biomacromolecules 14, 1529-1540.
575 576 577
Kaewprasit C., Hequet N., Abidi J.P., Gourlot J., (1998) Application of methylene blue adsorption to cotton fiber specific surface area measurement. Part I: methodology, J. Cott. Sci., 3, 164-173.
571 572 573 574
Kvien I., Tanem B.S., Oksman K., (2005) Characterization of cellulose whiskers and its nanocomposite by atomic force and electron microscopy, Biomacromolecules, 6, 3160-3165.
Li N., Bai R.B. (2005a) Copper adsorption on chitosan–cellulose hydrogel beads: behaviors and mechanisms, Sep. Purif. Technol. 42, 237–247.
584 585 586
Li N., Bai R.B., Liu C. (2005b) Enhanced and selective adsorption of mercury ions on chitosan beads grafted with polyacrylamide via surface-initiated atom transfer radical polymerization, Langmuir, 21,11780–11787.
587 588 589
Lin Y. F., Chen H.W., Chien P.S., Chiou C.S., Liu C.C. (2011) Application of bifunctional magnetic adsorbent to adsorb metal cations and anionic dyes in aqueous solution, J. Hazard. Mater., 185,1124–1130.
Liu C.C., Wang M.K., Li Y.S. (2005) Removal of nickel from aqueous solution using wine processing waste sludge, Ind. Eng. Chem. Res. 44,1438–1445.
592 593 594
Liu P., Sehaqui H., Tingaut P., Wichser A., Oksman K., Mathew A. P. (2014) Biobased nanomaterials for capturing silver ions (Ag+) from water via surface adsorption, Cellulose, 21, 449-461.
597 598 599 600
Ac ce p
579 580 581
Ma H., Burger C., Hsiao B.S., Chu B. (2011a) Ultra-fine cellulose nanofibers: new nano-scale materials for water purification, J. Mat. Chem. 21, 7507-7510.
Ma H., Burger C., Hsiao B.S., Chu B., (2012) Nanofibrous Microfiltration membrane based on cellulose nanowhiskers, Biomacromolecules, 13, 180186.
601 602 603
Ma H., Burher C. Hsiao B.S. Chu B. (2011b) Ultrafine polysaccharide nanofibrous membrane for water purification, Biomacromolecules, 12, 970976.
604 605 606 607
Mathew A.P., Laborie M- P, Oksman K. (2009), Cross-Linked Chitosan/Chitin crystal nanocomposites with improved permeation selectivity and pH stability. Biomacromolecules, 10, 1627-1632. 22 Page 22 of 25
Mathew A.P., Oksman K., Pierron D., Harmand M-F. (2012) Fibrous cellulose nanocomposite scaffolds prepared by partial dissolution for potential use as ligament or tendon substitutes, Carbohydrate Polymers, 87, 2291-2298.
611 612 613
Mikkonen K.S., Mathew A.P., Pirkkalainen K., Serimaa R., Xu C., Willfor S., Oksman K., Tenkanen M. (2010) Glucomannan composite film with cellulose nanowhiskers, Cellulose, 17, 69-81.
608 609 610
Min M., Shen L. Hong, G., Zhu M., Zhang Y., Wang X.,(2012) Micro-nano structure poly(ether sulfones)/poly(ethyleneimine) nanofibrous affinity membrane for adsorbtion of anionic dyes and heavy metals ions in aqueous solution. Chem. Eng. J. 197, 88-100.
619 620 621 622 623 624 625 626 627 628 629 630 631 632 633 634
Muzzarelli, R.A.A. (2012). Nanochitins and nanochitosans, paving the way to eco-friendly and energy-saving exploitation of marine resources. Poly. Sci.: A Compreh. Ref. 10, 153-164.
638 639 640 641
Muzzarelli, RAA; Morganti, P; Morganti, G; Palombo, P; Palombo, M; Biagini, G; Belmonte, MM; Giantomassi, F; Orlandi, F; Muzzarelli, C. (2007).Chitin nanofibrils / chitosan glycolate composites as wound medicaments. Carbohydrate Poly. 70, 274-284.
Narges N.; Algan C. Jacobs V, John M., Oksman K., Mathew A.P., (2014), Electrospun chitosan-based nanocomposite mats reinforced with chitin nanocrystals for wound dressing, Carbohydrate Polymers, 109, 7-15. Pavia D.L., Lampman G.M., Kriz G.S., (2002) Introduction to spectroscopy. A guide for students of organic chemistry; Thomson Learning: Mexico.
Ac ce p
635 636 637
615 616 617 618
Petersson L., Kvien I., Oksman K. (2007) Structure and thermal properties of poly(lactic acid)/cellulose whiskers nanocomposite materials. Compos. Sci. Technol. 67, 2535–2544.
Samir M.A., Alloin F., Dufresne A. (2005) Review of recent research into cellulosic whiskers, their properties and their application in nanocomposites field, Biomacromolecules, 6, 612–626.
642 643 644
Saxena A., Elder T.J., Pan S., Ragauskas A.J. (2009) Novel nanocellulosic xylan composite ﬁlm. Composites: Part B 40, 727–730.
23 Page 23 of 25
Shigemasa Y., Matsuura H., Sashiwa H., Saimoto H. (1996), Enzymatic degradation of chitins and partially deacetylated chitins, Int. J. Bio. Macromol., 18, 237-242.
650 651 652
Strand S., Sauperl O., Fras-Zemljic L., (2010) Cellulose fibers functionalized by chitosan: Characterization and application, Bioplymer, Magdy Elnashar (Ed), ISBN: 978-953-307-109.
646 647 648 649
Wesenberg D., Kyriakides I., Agathos S.N., (2003) White-rot fungi and their enzymes for the treatment of industrial dye effluents, Biotechnol. Adv., 22, 161–187.
654 655 656 657
Xiao S., Shen M., Guo R., Huang Q., Wang S., Shi X. (2010) Fabrication of multiwalled carbon nanotube-reinforced electrospun polymer nanofibers containing zero-valent iron nanoparticles for environmental applications, J. Mater. Chem. 20, 5700–5708.
658 659 660 661
Ac ce p
24 Page 24 of 25
662 663 Highlights
Chitosan membranes with cellulose nanocrystals (CNCs) as functional
Ultrafiltration membranes (≈ 250 m) with pores in the range of 13 - 17 nm
Homogeneous CNC dispersion, stabilized with chitosan in aqueous
Up to 99% removal efficiency for positively charged dyes and low water flux
Electrostatic interactions of surface functional group of CNCs with dyes
Ac ce p
25 Page 25 of 25